ANSI/AGMA C08 includes updated and extensively revised information from ANSI/AGMA B89 along with additional information needed to achieve . Download ANSI-AGMA B Gear Materials and Heat Treatment Manual. Index of AGMA Standards and Information Sheets by Number. 1 ANSI/AGMA B89 Gear Materials and Heat. Treatment Manual.
|Published (Last):||13 January 2008|
|PDF File Size:||1.2 Mb|
|ePub File Size:||3.75 Mb|
|Price:||Free* [*Free Regsitration Required]|
ANSI-AGMA 2004-B89-1995 Gear Materials and Heat Treatment Manual
The controlled porosity in powder metal parts permits their impregnation with oil to provide a self lubricating part, especially for the internal type of gears.
Lower core hardness does not support the hard, thin case as well as higher core hardness. It may be advisable to specify by use of photomicrographic standards both 2004-b9 and nonacceptable phase distributions in the gear rim section. Excessive tooth distortion and a loss of core ductility can also occur. Repairs in the rim tooth portion and other critical load bearing locations should be performed only prior to heat treatment.
Tables in the appropriate reference are available as guidelines for the effect of tempering temperature on agam. Crowning is more desirable from a tooth loading standpoint. Saturation is defined as that point at which doubling the time of exposure will result in no more than a 10 percent increase in arc height.
Only the noncritical top lands of teeth are not hardened. Parts are rotated when encircling coils are used.
Carburizing and carbonitriding can be performed, but products with a density under 6. During both spin flame and spin induction hardening, the entire tooth cross section is often hardened to the specified depth below the roots of 2004-h89. Nitrided case depth is defined as the depth at which the hardness is equivalent to percent of the measured core hardness.
However, even with perfectly uniform sections, parts can easily crack if made 200-4b89 highcarbon, highhardenability steels and the quench is too severe. Wrought steel is anisotropic, however, meaning that the mechanical properties tensile ductility and fatigue and impact strength vary according to the direction of hot working or inclusion flow during forming see Fig The load in kilograms force listed in Table should be used.
The recommended test bar diameter for bevel gearing is to be approximately equal to the inscribed diameter of the normal tooth thickness at mid face width. Surface hardness is limited by the concentration of hard nitride forming elements in the alloy and the core hardness of the gear.
Tanaka Nippon Gear R. Finer pitch gearing generally utilizes encircling coils with power provided by high frequency vacuum tube units. For additional information on wrought steel manufacture and steel making refining practices, reference should be made to the following sources: The amount and direction of growth or movement should be determined for each part by dimensional analyses both prior to and after nitriding.
Same as above; however, thin sections or sharp corners can represent a crack hazard. This standard has been updated to reflect current technology in the area of steel making and heat treatment, and edited to include cross references to relevant AGMA standards and information sheets.
Item Detail – ANSI/AGMA C08 (reaffirmed March )
Parts which are to be nitrided should have the following specified: The minimum hardness, using a kg load, shall be 80 HB for static chill and centrifugal chill castings, and 70 HB for sand castings. Normalizing results in higher hardness than annealing, with hardness being a function of grade of steel and the part section thickness.
Density is the most significant characteristic of powder metal materials. When four hardness tests are required, two tests should be made on the cope side, one over a riser and the other approximately degrees away between risers, and two tests on the drag side 90 degrees away from the tests on the cope gama. Spin hardening is more amga for smaller gears. Through hardening does not imply that the part has equivalent hardness throughout the entire cross section.
Controls should be checked and calibrated at regular intervals. The advantages and limitations as described herein should be fully understood before specifying carbonitriding for industrial gearing. 2004-b899 case depths are generally specified for carbonitriding than is agmx for production carburizing.
Gear blanks can also be quenched and tempered. Open die forgings may be specified to be upset forged to increase center densification.
Hardenability is constant for a given steel composition; however, hardness will vary with the cooling rate. Forgings reduce machining time, and are available in a wide range of sizes and grades. Repair welds in the tooth area should be performed only with the approval of the gear manufacturer.
Sueyoshi Tsubakimoto Chain M. Contour induction amga results in case depth at the root to be approximately 60 percent of the depth at the pitchline due to mass quench and hardenabiltiy effect.